# a method for Discrete Material and Thickness Optimization

## Comments

## Transcription

a method for Discrete Material and Thickness Optimization

Aalborg Universitet DMTO – a method for Discrete Material and Thickness Optimization of laminated composite structures Sørensen, Søren Nørgaard; Sørensen, Rene; Lund, Erik Published in: Structural and Multidisciplinary Optimization DOI (link to publication from Publisher): 10.1007/s00158-014-1047-5 Publication date: 2014 Document Version Early version, also known as pre-print Link to publication from Aalborg University Citation for published version (APA): Sørensen, S. N., Sørensen, R., & Lund, E. (2014). DMTO – a method for Discrete Material and Thickness Optimization of laminated composite structures. Structural and Multidisciplinary Optimization, 50(1), 25-47. DOI: 10.1007/s00158-014-1047-5 General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights. ? Users may download and print one copy of any publication from the public portal for the purpose of private study or research. ? You may not further distribute the material or use it for any profit-making activity or commercial gain ? You may freely distribute the URL identifying the publication in the public portal ? Take down policy If you believe that this document breaches copyright please contact us at [email protected] providing details, and we will remove access to the work immediately and investigate your claim. Downloaded from vbn.aau.dk on: august 13, 2017 DMTO – a method for Discrete Material and Thickness Optimization of laminated composite structures Søren N. Sørensen1 , René Sørensen2 , and Erik Lund3 1,2,3 Department of Mechanical and Manufacturing Engineering, Aalborg University, Fibigerstraede 16, DK-9220 Aalborg East, Denmark, 1 [email protected], 2 [email protected] May 2014 Abstract by the simultaneous determination of material distribution and thickness variation. The method is labelled Discrete Material and Thickness Optimization (DMTO), being an immediate extension of the original DMO method by Stegmann and Lund (2005). Mass minimization reduces material expenses and issues related to the net weight of the structure. Mass is minimized subject to constraints on the following structural criteria; buckling load factors, eigenfrequencies, and limited displacements. Furthermore, series of so-called manufacturing constraints (MC’s) are considered as a means to fulfill experience based design guidelines or rules for laminated composite structures. This paper presents a gradient based topology optimization method for Discrete Material and Thickness Optimization of laminated composite structures, labelled the DMTO method. The capabilities of the proposed method are demonstrated on mass minimization, subject to constraints on the structural criteria; buckling load factors, eigenfrequencies, and limited displacements. Furthermore, common design guidelines or rules, referred to as manufacturing constraints, are included explicitly in the optimization problem as series of linear inequalities. The material selection and thickness variation are optimized simultaneously through interpolation functions with penalization. Numerical results for several parameterizations of a finite element model of a generic main spar from a wind turbine blade are presented. The different parameterizations represent different levels of complexity with respect to manufacturability. The results will thus give insight into the relation between potential weight saving and design complexity. The results show that the DMTO method is capable of solving the problems robustly with only few intermediate valued design variables. 1 As the DMTO name suggests, the laminate thickness should preferably add up to a discrete number of plies with predefined thicknesses. The number of plies must naturally be able to vary throughout the structure to facilitate mass reduction. The material selection is conducted among a discrete set of material candidates, and should preferably result in a distinct choice rather than a mixture between two or more candidates. Intermediate valued, continuous variables, are penalized as the means to obtain the preferred discreteness. This classical density approach is elaborated in the following section. The candidates may consist of any material, as it is merely required to input the effective constitutive properties and density. It is thus possible to choose among the same orthotropic material with different fiber orientations, biax-angle fiber materials, foam and wood materials, or even customized Non Crimp Fabrics (NCF’s) and prepregs. This selection among a discrete set of candidates resembles the current production technology of several laminated composite structures. In the wind turbine industry, the material candidates are typically placed, rolled out, or stacked in a mold where they are processed using vacuum infusing techniques. Introduction Today, laminated composites are used in a wide variety of weight critical products, ranging from recreational items like badminton rackets and mountain bikes, to large industrial structures such as airplanes and wind turbines. Designing such structures is not a straightforward task as it requires considerations regarding e.g., available materials, demands for performance, manufacturing methods, and common design guidelines or rules, referred to as manufacturing constraints. As a consequence of these criteria, the design process is typically iterative and time consuming. From an engineering perspective, one way of systematically addressing such a design process is to use a suitable optimization method. In this paper, we present a gradient based topology optimization method for mass minimization of laminated composite structures Material optimization on basis of a discrete set of candidates for structures with constant laminate thickness has attracted much attention in the last decades. Most contributions on this topic have been summarized in Ghiasi et al. (2009). In the original DMO method, the 1 Most approaches on variable laminate thickness optimization divide the optimization process into multiple phases where thickness and material determination are handled separately. Liu et al. (2011) presented a two phase or bilevel method for minimizing the mass of composite wing panels subject to strain constraints. In the first phase, the number of {−45◦ , 0◦ , 45◦ , 90◦ } plies was determined, and in the second phase a GA was utilized to shuffle the placement of plies in order to accommodate common design rules used in the aerospace industry. The approach applied by Altair Engineering in the commercial software OptiStruct relies on three distinct phases, see Zhou et al. (2011) and Zhou and Fleury (2012). Phase I concerns the conceptual ply layout; Phase II determines the specific number of plies; Phase III determines the final stacking sequence of the laminate, taking into account performance demands and the previously mentioned manufacturing constraints. The method proposed in this paper considers thickness and material determination simultaneously, explicitly taking into account performance demands and manufacturing constraints throughout the process. The addition of manufacturing constraints in laminate design optimization has attracted more attention as the optimization methods have evolved. Manufacturing constraints represent common design guidelines or rules formulated to e.g., reduce the risk of local failure in the structure. These failure modes are typically associated with out-of-plane stresses that are not captured with a sufficient level of detail when using standard shell elements in a finite element context. In order to capture these effects, a 3D-solid finite element model could be applied. Such detailed modeling is, however, seldom applied in optimization frameworks, given a substantial computational time. Hence, manufacturing constraints serve as an effective way of implicitly considering these effects, and thus obtain designs that require less time for manual post-processing. Generally, the constraints typically found in the literature have their origins in the aerospace industry, see Kassapoglou (2010). Manufacturing constraints can furthermore be used to limit the complexity of the optimized design, thus making it possible to achieve a higher degree of manufacturability. In this work, four common manufacturing constraints, denoted MC1-MC4, introduced in the previous work by Sørensen and Lund (2013), are considered. MC1 is not an explicit constraint as it is related to the design parameterization. In short, MC1 concerns the possible arrangement or grouping of small finite element domains into larger domains, adequate for the allowable variation in both candidate selection and thickness. MC2 explicitly limits the thickness variation rate between adjacent design regions to reduce the risk of delamination. Costin and Wang (1993) formulated a similar constraint in the case where the individual laminae thicknesses are applied as continuous design variables. MC3 limits the number of identical contiguous selection of a distinct material candidate was achieved by balancing the different design variables such that an increase in one would automatically decrease remaining ones, see Lund and Stegmann (2005). More recently, Hvejsel et al. (2011) considered alternative strategies for discrete multi-material stiffness optimization and proposed series of linear equality constraints to prevent the total sum of the candidate design variables from exceeding unity within each design domain. In order to obtain discrete designs, i.e., the distinct selection of exactly one of the candidates, the authors furthermore proposed a quadratic penalty constraint to gradually force the design variables to their discrete bounds. As an alternative to this non-linear penalty constraint, Hvejsel and Lund (2011) formulated multi-material variations of the SIMP and RAMP interpolation schemes, see Bendsøe (1989) and Stolpe and Svanberg (2001), respectively. As an alternative to the DMO schemes, Bruyneel (2011) introduced the Shape Functions with Penalization (SFP) scheme. The SFP scheme is based on the shape functions of a quadrangular first order finite element, using only two natural coordinates to interpolate between four material candidates. The method was later extended to also include three and eight node elements, see Bruyneel et al. (2011). Gao et al. (2012) proposed a Bi-valued Coding Parameterization (BCP) scheme which distinguishes itself from SFP schemes in that it does not have a limit on the number of applied material candidates. SFP and BCP schemes reduce the number of required design variables compared to DMO schemes. We finally mention Kennedy and Martins (2013) that proposed a series of non-linear equality constraints, which were added as a penalty term to the objective function, thereby penalizing intermediate valued design variables. The above mentioned methods are capable of optimizing the material distribution throughout a laminated composite with constant total thickness. Thus, allowing for determining either an optimum stacking sequence or a sandwich design throughout the predefined and fixed number of layers. Most methods have traditionally been demonstrated on mass constrained minimization of compliance. However, recent advances within the field have likewise been demonstrated on eigenfrequency problems, see e.g., Lund and Stegmann (2005) and Niu et al. (2010), and also problems considering buckling load factors have been attracting more attention, see e.g., Lund (2009) and Kennedy and Martins (2013). Literature concerning optimization of multilayered laminated composite structures with variable total thickness is more limited. Ghiasi et al. (2010) reviews work on variable stiffness designs, with only few references concerning variable thickness. Manne and Tsai (1998) utilized plydrop tapering for thickness optimization of symmetric layups to avoid warping. Toropov et al. (2005) applied a Genetic Algorithm (GA) to minimize the mass of a monolithic composite wing rib model using discrete fiber orientations and the number of plies as design variables. 2 layers through the thickness to reduce the risk of matrix cracking. This type of constraint has been investigated by e.g., Le Riche and Haftka (1993), Liu et al. (1999), Toropov et al. (2005), and Liu et al. (2011) in the context of stacking sequence optimization with GA’s. Also, Bruyneel et al. (2012) included this constraint for discrete material optimization with constant thickness. MC4 prevents intermediate void from appearing through the thickness of the laminate. MC1-MC4 are all formulated as linear constraints, which makes them efficient to fulfill for the optimizer. The constraints are elaborated in Section 2.3. Several other manufacturing constraints occur in the literature such as requirements for e.g., symmetric and balanced laminates, minimum proportion or presence of candidates, and so-called adjacency constraints or blending rules to limit the in-plane change in fiber orientation, see e.g., Seresta et al. (2007), Kassapoglou (2010), Zein et al. (2012), Bruyneel et al. (2012), and Kennedy and Martins (2013). In spite of the clear relevance of the above mentioned manufacturing constraints, these particular constraints are not explicitly considered in the DMTO method to be presented here. The formulation and inclusion of such constraints are hence left for future work on the DMTO method. Other potential manufacturing constraints which would be of interest would be a type of sandwich constraint, ensuring that core material is always enclosed by layers of fiber material. The necessity of one such sandwich constraint is discussed in Section 5. As mentioned, manufacturing constraints are mainly included to reduce the risk of out-of-plane failure modes. In-plane failure modes could potentially be monitored by including local strength criteria such as e.g., max stress and max strain constraints or other criteria such as the Tsai-Wu failure criterion, see Tsai and Wu (1971), Kim et al. (1994), and Groenwold and Haftka (2006). In the context of topology optimization with isotropic materials, stress constraints have been investigated by Duysinx and Sigmund (1998) and more recently by Le et al. (2010), Parı́s et al. (2010), and Bruggi and Duysinx (2012). The formulation and inclusion of local constraints within gradient based, multimaterial topology optimization is currently being investigated by e.g., Lund et al. (2013), but is not yet a mature technology. Despite of the obvious relevance, local criteria are not considered here but left for future work. The method proposed in this work is a continuation of the work by Sørensen and Lund (2013) who presented a novel method for simultaneous determination of material distribution and thickness variation of multilayered laminated composite structures. The preceding method was demonstrated on simply parameterized monolithic laminated plates with various boundary conditions, where the objective was to minimize compliance subject to a mass/volume constraint and manufacturing constraints MC1-MC4. Compared to the preceding work, we are now considering multi-material topology optimization. Likewise, we change focus from minimum compliance optimization to minimizing mass subject to the following structural performance constraints; buckling load factors, eigenfrequencies, and limited displacements. Mass minimization is viewed as an industrially more relevant problem, as the mass can be directly related to the cost of the final product. Together with the manufacturing constraints MC1-MC4, this is altogether constituting a far more difficult problem. The additional difficulties arise from the presence of the non-linear and non-convex structural constraint functions. In order to manage these difficulties, we present a new procedure for obtaining near discrete design. The capabilities of the DMTO approach are demonstrated on several parameterizations of a finite element model of a generic main spar from a wind turbine blade. The different parameterizations show the flexibility of the proposed method, but also represent different levels of complexity with respect to manufacturability. The results will thus give insight into the relation between potential weight saving and design complexity. It is noticed that DMTO results should not be viewed as final designs, ready to manufacture, as the final design may still need some amount of manual post-processing despite the inclusion of certain manufacturing constraints. There are several reasons for this, of which one is related to the assumption that adjacent layers with different fiber orientations are perfectly bonded. These regions are typically manufactured by introducing a certain amount of in-plane overlap between the two fiber materials and require detailed analysis. Likewise, the optimized structure may be part of a larger assembly of other sub-structures. Hence, jointing and other detailed considerations with regards to assembly have to be done post to the optimization procedure. Thus, the optimized results should rather serve as a vital source of inspiration for thickness variation and stacking sequences throughout the entire structure, taking into account the complexity of elastic couplings and demands on structural performance as well as manufacturing constraints. The paper is organized as follows. Section 2 explains the DMTO method in detail, covering areas regarding the design parameterization, the applied density approach, the considered manufacturing constraints MC1-MC4, the mathematical formulation including sensitivity analysis, the Sequential Linear Programming (SLP) approach, and a simple rounding technique to finalize the optimized results. Section 3 introduces several numerical examples concerning a finite element model of a generic main spar from a wind turbine blade. Numerical results are presented in Section 4 and discussed in Section 5. The paper is finalized with conclusions in Section 6. 3 Step 2 (Ωdl ) Step 1 (FE) Step 4 (x jc ) Step 3 (ρi ) ρ5 Ω13 x5c Ω33 Ω23 ρ6 Ω43 1 2 4 3 5 Ω12 Ω32 Ω22 x3c ρ2 ρ3 ρ4 Ω42 x4c z Ω11 y x Ω31 Ω21 x1c ρ1 x2c Ω41 Figure 1: The design parameterization takes place in 4 steps. Step 1 concerns the finite element discretization. Step 2 concerns the arrangement into sub-domains, Ωdl . Step 3 and Step 4 concern the parameterizations into geometry domains, ρi , and candidate domains, x jc , respectively 2 The DMTO method in Step 2, where the designer must settle on a sufficiently detailed level for such variations and transitions, common for all layers. Hence, Step 2 concerns the arrangement of finite elements into a number of sub-domains Ωdl , which are identically shaped for all layers covered by the sub-domain, where indices d = 1, 2, . . . , nd and l = 1, 2, . . . , nl denote sub-domain number and layer number, respectively. Consequently, the sub-domains are coincident with the boundaries of at least one of the finite elements and do not overlap each other. The sub-domains constitute the building blocks for the subsequent parameterization into domains that are directly associated with the design variables. For this illustrative example, finite elements 1 and 2 have been collapsed into the sub-domain d = 1, and the remaining elements have been assigned as sub-domains d = {2, 3, 4}. Step 3 concerns the adequate parameterization for the laminate thickness variation. For this purpose we introduce the so-called topology variables ρi ∈ [0, 1] with the desirable limit value interpretation 1 if there is material in geometry domain i ρi = (1) 0 otherwise 2.1 Design parameterization Out of generality, this work clearly distinguishes between the initial finite element discretization and following arrangement into domains limiting the complexity of the geometric outcome, and domains limiting the complexity of the possible candidate distribution. As the results in Section 4 will demonstrate, the design parameterization significantly affects both performance and complexity of the optimized designs. The designer must from the very beginning keep in mind that the design parameterization should reflect adequate limits of complexity in manufacturing, thereby making it possible to realize the optimized design given an acceptable level of post-processing. The design parameterization takes place in four steps as exemplified in Fig. 1. Step 1 of Fig. 1 concerns the finite element (FE) discretization into an appropriate number of Equivalent Single Layer (ESL) shell elements all with an identical number of layers of uniform thickness. In the figure, five elements are shown, each having three layers of uniform thickness. The appropriate number of elements may be determined based on a convergence study, considering all optimization criteria. The necessary finite element discretization may, however, often be too fine for the acceptable level of the thickness variation and transitions in fiber orientation or different material selection that is about to take place. This problem is considered where the index i = 1, 2, . . . , ni denotes the so-called geometry domain number. The geometry domains are coincident with the boundaries of at least one of the subdomains. The geometry domains may principally overlap each other from layer to layer as seen in Fig. 1; it is up 4 c = 1 (E1 ) to the manufacturing constraints to ensure e.g., prevention of intermediate void. Application of a single topology variable for the bottom layer l = 1 ensures a constant thickness throughout governed by the value of ρ1 . In Step 4, the acceptable level for jointing adjacent fiber mats with different orientations, different biax-angle plies, NCF’s, or even different materials, is defined. For this purpose we introduce the so-called candidate variables x jc ∈ [0, 1] with the desirable limit value interpretation 1 if cand. c is chosen in cand. domain j x jc = (2) 0 otherwise c = 2 (E2 ) c = 3 (E3 ) (Foam) where index j = 1, 2, . . . , n j denotes the so-called candidate domain number and index c = 1, 2, . . . , nc denotes the candidate number. A candidate c represents a unique set of material properties for the constitutive tensor Ec ∈ R6×6 . Hence, some candidates may represent differently oriented UniDirectional (UD) fiber mats, while other candidates may represent biax-angle plies, NCF’s, or isotropic materials such as a lightweight foam in case of designing sandwich structures. Hence, the method supports any set of physical constitutive properties. Similar to the geometry domains ρi , the candidate domains x jc may likewise overlap each other from layer to layer as seen in Fig. 1. Figure 2 illustrates a potential outcome of the considered example where the constitutive properties characterizing a Glass Fiber Reinforced Polymer (GFRP) ±45◦ biax-angle ply represents the material candidate c = 1 and hence E1 , an isotropic foam material represents candidate c = 2 (E2 ), and a UD GFRP oriented at −45◦ represents candidate c = 3 (E3 ). The design parameterization of Fig. 1 and the outcome illustrated in Fig. 2 are used to exemplify the formulation and effect of certain manufacturing constraints in succeeding sections. Presence of exactly one candidate must naturally ensure absence of remaining ones. In this work we ensure this coherence explicitly through the series of linear equality constraints nc X x jc = 1 ∀ j y/90◦ x/0◦ In (4), careful bookkeeping keeps track of proper association between finite element discretization versus design variable location. We introduce a product of RAMP interpolation schemes to facilitate difference in geometric variation and candidate distribution while making binary variables attractive. c n X x jc ρi Eel = E0 + ∆Ec 1 + p(1 − ρi ) c=1 1 + p(1 − x jc ) (3) 2.2 Density approach The constraints (3) in combination with continuous candidate variables introduce the risk of non-manufacturable, non-physical pseudo candidates if linearly summarized to describe the effective constitutive properties Eel for all layers of all elements e as x jc Ec (5) where ∆Ec = Ec − E0 with E0 representing void such that Ec − E0 ≻ 0 and E0 ≻ 0. In (5), p ≥ 0.0 is a penalization power. Notice that variables ρi and x jc are subject to identical penalization, found appropriate by experience. We favor the RAMP interpolation scheme by Stolpe and Svanberg (2001) after Rietz (2001) because of non-zero sensitivities even for zero valued design variables for all penalization powers. Other schemes exist and are known to work as well; it is a matter of preference. Equivalent penalization between the RAMP scheme and the well-known SIMP scheme by Bendsøe (1989) is treated in Hvejsel and Lund (2011). Notice that the products ρi x jc ensure candidate continuity within the pre-defined candidate domains while having the freedom to introduce regions with void through topology variable scaling. This facilitates an outcome as illustrated in Fig. 2, subject to the parameterization of Fig. 1. Here, the candidate domain x5c , covering subdomains {Ω13 , Ω23 , Ω33 , Ω43 }, has settled on the specific biax-angle candidate c = 1, but since the topology variable ρ6 = 0, only sub-domain Ω13 where ρ5 = 1 appears. The association between sub-domains Ωdl , geometry do- It is noticed that (3) is of no importance for obtaining the desirable 0/1 designs; this is left for penalization of intermediate values through the density approach. Eel = θ Figure 2: Top: Potential outcome of an example, parameterized as illustrated in Fig. 1. Bottom: Any unique set of material properties for the constitutive tensor Ec may represent a candidate c such as for instance a foam type (left) or GFRP UD fiber mats (right), characterized by the fiber orientation θ c=1 nc X (GFRP) (4) c=1 5 2.3 Manufacturing constraints mains ρi , candidate domains x jc , and the corresponding design variable value distribution for the considered example in Fig. 2 appears in (6) in case the number of candidates is limited to those three introduced in Fig. 2 (top), i.e., nc = 3. Practical design guidelines or rules, referred to as manufacturing constraints in this work, occur frequently in the literature. As described in the introduction, manufacturing constraints are typically associated with different outof-plane failure modes and may be implemented in vari ous ways. In this work, we explicitly include a variety of x1c = { 0 1 0 } ρ1 = 1 Ω11 x = { 0 1 0 } ρ = 1 Ω manufacturing constraints as linear inequalities to accom3c 2 12 x = { 1 0 0 } ρ = 1 Ω modate demands on manufacturability. The linear formu 5c 5 13 x2c = { 0 0 1 } ρ1 = 1 Ω21 lations are highly attractive and possible to achieve for x3c = { 0 1 0 } ρ2 = 1 Ω22 most manufacturing constraints. Explicit inclusion from x5c = { 1 0 0 } ρ6 = 0 Ω23 the very beginning is the key to the simultaneous determi ←→ (6) ←→ nation of geometry, i.e., the variation in thickness, and x1c = { 0 1 0 } ρ1 = 1 Ω31 x = { 0 1 0 } ρ = 1 Ω the proper candidate choice from a predefined, distinct 3c 3 32 x5c = { 1 0 0 } ρ6 = 0 Ω33 set. Formulations of the manufacturing constraints are x2c = { 0 0 1 } ρ1 = 1 Ω41 deemed most easily comprehensible when exemplified as ∗ x4c = { 1 0 0 } ρ4 = 0 Ω42 below with basis in the parameterization presented in Fig. 1 and the resulting outcome in Fig. 2. Correct formulation Ω43 ρ6 = 0 x5c = { 1 0 0 } relies on proper bookkeeping between the parameterizations applied in Steps 2 − 4, exemplified in (6) for the The star on x∗4c denotes that the candidate material selec- outcome in Fig. 2. tion in this particular case is insignificant because the associated geometry domain is empty, i.e., ρ4 = 0. The design variable value distributionn for x∗4c must ocomply with 2.3.1 Accommodations for allowable candidate and thickness variation (MC1) 1 1 1 (3) but could as such be x∗4c = or any other 3 3 3 combination with no influence on the effective constitu- MC1 concerns the possible arrangement or grouping of tive properties, given (5) with ρ4 = 0. small finite element domains into larger domains, adeWith the stiffness parameterization (5), one could quate for the allowable variation in both candidate seleclikewise determine how, for instance, the well-known tion and thickness. These latter domains are directly asMesserschmitt-Bølkow-Blohm (MBB) beam, see e.g., sociated with the design variables as part of the design Olhoff et al. (1991) or Bendsøe and Sigmund (2003), parameterization, see Steps 3-4 in Fig. 1. It is thus poswould appear, if the entire domain should settle on a spe- sible to e.g., ensure sufficiently large areas with identical cific candidate from a distinct set while having the pos- candidate selection to support standard roll widths for fisibility to mix with void through topology variable scal- brous material. Hence, MC1 reflects adequate limits of ing. The outcome would indeed be quite easily manufac- complexity with regards to the available production methods, thereby making it possible to realize the optimized turable. designs with quite little post-processing. An approach as (5) where stiffness is determined through interpolation schemes with penalization, but mass is not, making non 0/1 variable values uneconomi- 2.3.2 Constraints on thickness variation rate (MC2) cal, is generally referred to as the density approach, and is used extensively throughout the literature on structural Let S ∈ N denote the allowable difference in the total topology optimization, see Bendsøe and Sigmund (2003). number of plies between adjacent geometry domains, The density approach is known to work particularly well ρi . Constraints to govern the acceptable thickness for mass constrained minimization of compliance, but variation rate e-merge on basis of systematical comparmay nevertheless fail at obtaining pure 0/1 designs for ison between topology variable summation through the various reasons. The difficulties of obtaining binary de- thickness of all adjacent design domains Ωdl , taking into signs are increased in this work, primarily due to the account, however, possible reduction because certain presence of sensitivities with both operational signs. For topology variable pairs may cancel out each other, caused this reason, we finalize the optimized designs with simple by the fact that geometry domains can overlap several rounding to binary values, elaborated in Section 2.6. To sub-domains. This gives rise to four linear inequalities assess the quality of the optimized designs prior to this for the considered example. rounding, we will introduce so-called measures of nondiscreteness in Section 2.5. The finite element formu- Ω1l vs Ω2l : lations of the considered criteria functions are treated in ρ✚ ρ✚ ρ❩ −S ≤ (✚ ρ❩ (7a) 2 + ρ5 ) − (❩ 1 +✚ 1 +❩ 2 + ρ6 ) ≤ S Section 2.4. 6 Ω1l vs Ω3l : ρ✚ ρ❩ −S ≤ (✚ 1 + ρ2 + ρ5 ) − (❩ 1 + ρ3 + ρ6 ) ≤ S ensure that topology variable values of upper layers do not exceed those of lower contiguous layers such as for instance ρ5 ≤ ρ2 ≤ ρ1 , see Fig. 1. In the preceding work by Sørensen and Lund (2013) it was, however, concluded that series of such straightforward constraints were insufficient at preventing so-called density bands where the topology variables settled on the same intermediate value throughout the thickness regardless of the penalization level. For this reason we apply the same modified constraints to prevent intermediate void as suggested in Sørensen and Lund (2013), thereby ensuring an acceptable transition between contiguous topology variables throughout the thickness. The constraints emerge systematically on basis of the sub-domain arrangement Ωdl followed by removal of repeated constraints because of potentially larger geometry domains ρi . This gives rise to seven linear inequalities for the considered example. (7b) Ω2l vs Ω4l : ρ✚ ρ✚ ρ❩ −S ≤ (✚ ρ❩ 6 ) − (❩ 1 + ρ2 + ✚ 1 + ρ4 + ❩ 6) ≤ S (7c) Ω3l vs Ω4l : ρ✚ ρ✚ ρ❩ −S ≤ (✚ ρ❩ 6 ) − (❩ 1 + ρ3 + ✚ 1 + ρ4 + ❩ 6) ≤ S (7d) The outcome in Fig. 2 is feasible for all S ≥ 1. 2.3.3 Constraints on contiguity (MC3) Let Pc(U D) denote the unique set of indices c that concerns UD fiber material candidates. The constraints on contiguity impose a limit on the maximum allowable number of contiguous identical UD fiber material candidates to avoid e.g., matrix cracking failure. Hence, non UD candidates are not subject to the following constraints. Let CL ∈ N denote the contiguity limit. In case CL = 1, the candidate selection for all contiguous Ωdl pairs must be constrained. However, since the candidate domains are larger than or equal to the sub-domains, we see that a number of constraints repeat themselves for which reason the redundant ones are erased for efficiency. Concerning Ω1l : ρ2 ≤ f (ρ1 , T ) (9a) ρ5 ≤ f (ρ2 , T ) (9b) Concerning Ω2l : ρ2 ≤ f (ρ1 , T ) (9c) ρ6 ≤ f (ρ2 , T ) (9d) Concerning Ω3l : Concerning Ω1l : x1c + x3c ≤ CL ∀c ∈ Pc(U D) (8a) x3c + x5c ≤ CL ∀c ∈ Pc(U D) (8b) ρ3 ≤ f (ρ1 , T ) (9e) ρ6 ≤ f (ρ3 , T ) (9f) Concerning Ω4l : Concerning Ω2l : ρ4 ≤ f (ρ1 , T ) x2c + x3c ≤ CL ∀c ∈ x3c + x5c ≤ CL ∀c ∈ Pc(U D) Pc(U D) Concerning Ω3l : x1c + x3c ≤ CL ∀c ∈ Pc(U D) x3c + x5c ≤ CL ∀c ∈ Pc(U D) Concerning Ω4l : (9g) (8c) ρ6 ≤ f (ρ4 , T ) (9h) (8d) In (9) the right-hand sides f (ρi , T ) denote functions depending upon density values of contiguous lower layers and a threshold value T to control the transition, given as (8e) T if ρi < (1 − T ) 1−T ρi (10) f (ρ , T ) = i 2T −1 1−T (8f) else T ρi + T In Sørensen and Lund (2013), the threshold value T = 0.10 was found appropriate and is used in this work as x2c + x4c ≤ CL ∀c ∈ Pc(U D) (8g) well. Because the topology variable ρ4 = 0 for the examx4c + x5c ≤ CL ∀c ∈ Pc(U D) (8h) ple in Fig. 2, ρ6 must likewise be equal to zero to fulfill (9h), thereby efficiently preventing intermediate void. For the example in Fig. 2, only c = 3 is a UD fiber material candidate; hence Pc(U D) = {3}. 2.4 Mathematical formulation of the optimiza- tion problem 2.3.4 Preventing intermediate void (MC4) In this work, we want to minimize the total mass, subIntermediate void must be prevented in order to support ject to constraints on buckling load factors, eigenfrequencommon manufacturing techniques relying on vacuum cies, displacements, and the linear manufacturing coninfusion. To facilitate this, it principally suffices to straints presented in Section 2.3. We apply the Nested 7 ANalysis and Design (NAND) approach, see for instance a maximum allowable displacement uo . Elastic couplings Arora and Wang (2005), to solve the optimization prob- may necessitate displacement constraints on several nodal lem that appears in (11). DOF’s, contained in a corresponding set, denoted by Pu . Given the NAND approach, the global displacement vecmin m (Mass) (11a) tor u is determined prior to every optimization iteration ρi ,x jc from the static equilibrium equations (b) s.t. λ(b) k = 1, 2, . . . , n(b) (Buck) (11b) λ k ≥λ λ(kf ) ≥ λ( f ) k = 1, 2, . . . , nλ( f ) u |uo | ≤ uo ∀o ∈ P (MC’s) (Freq) (Disp) (11c) K0 u = f (11d) written in residual form as (15) (11e) r(u, ρ , x ) = K u − f = 0 i jc 0 (16) (11f) where f denotes the load applied to the non-restrained x jc ∈ [0, 1]∀ ( j, c) (11g) nodes and r is the residual. Besides the total mass m in (12) that is clearly a function of the design variables ρi and x jc , it must by now be noticed that this is likewise In (11a), m denotes the total mass, determined as the case for both K0 and Kσ due to the dependence on nc X X the effective constitutive properties (5). It is neither trivial m= ρi Vdl x jc ̺c (12) nor obvious where to most efficiently penalize this design d,l c=1 variable dependence. In this work, however, we reserve taking into account proper association between indices dl, penalization p for the linear stiffness matrix part K0 only, i, and j, as exemplified in (6). Vdl denotes the volume i.e., of sub-domain Ωdl , and ̺c is the material density of can(17) didate c. In (11b), λ(b) denotes the minimum allowable K0 = f (p) , Kσ , f (p) , m , f (p) (b) th buckling load factor. λk denotes the k eigenvalue, i.e., The numerical results in Section 4 will demonstrate the buckling load factor, out of the considered n(b) λ eigenval- efficiency of this approach, and alternative penalization is ues, assumed ordered by magnitude such that λ(b) 1 is the left for future work. See for instance Lindgaard and Dahl lowest positive eigenvalue. The advantage of including (2012) for penalization approaches concerning topology (f) n(b) λ and nλ eigenvalues in the optimization problem in- optimization of geometric non-linear compliance and stead of only including the lowest eigenvalue is that crossbuckling. ing eigenvalues (mode switching) during the optimization process are taken into account. In the examples considered the lowest 10 buckling load factors and eigenfre- 2.4.1 Design sensitivity analysis quencies are included. Based on the displacement field, Let zi represent all design variables ρi and x jc in the folthe stress stiffening effects due to the mechanical loading lowing, where the index i = 1, 2, . . . , ni n j nc . This subseccan be evaluated by computing the initial stress stiffness tion describes how we conduct analytical, computationmatrix, also termed the geometric stiffness matrix, Kσ , ally efficient adjoint Design Sensitivity Analysis (DSA) and the linearized buckling problem can be established as (f) dλk du , and distinct eigenvalues, and of displacements, dz dz i i (b) (b) (b) = 0 , k = 1, 2, . . . , n (13) Φ K K0 + λ(b) σ dλ λ k k k dzi , concerning eigenfrequencies and buckling load factors, respectively. Notice that this work is limited to DSA where Φ(b) k denotes the corresponding eigenvector of displacements and K0 is the linear stiffness matrix. The no- of distinct eigenvalues as opposed to the more complitation in (11c) is similar but with superscript ( f ) denot- cated case where two or several eigenvalues attain exactly (f) ing frequency. Hence, ω2k = λk is the kth squared, un- the same value, known as repeated or multiple eigenvaldamped, free, natural eigenfrequency, determined from ues. For details on this latter case see e.g., Seyranian et al. (1994) or Lund (1994). DSA of the objective function the free vibration analysis problem mass in (12), dm dzi , is straightforward and omitted. (f) (f) (f) du K0 − λk M Φk = 0 , k = 1, 2, . . . , nλ (14) The displacement sensitivities dz can be computed usi ing the direct differentiation approach, i.e., the static equi(f) where Φk denotes the corresponding eigenvector, i.e., librium equations (15) are differentiated with respect to a nodal amplitudes, and M is the consistent global mass design variable zi as matrix. Eigenvalues are again assumed ordered by magnitude. In (11d), |uo | denotes the absolute displacement K du = ∂ f − ∂K0 u (18) 0 dzi ∂zi ∂zi of the nodal degree of freedom (DOF) o, constrained by ρi ∈ [0, 1] ∀ i 8 where the load sensitivities ∂ f /∂zi are zero for the DMTO where the eigenvectors have been Kσ -orthonormalized, design variables used, unless volume forces are consid- such that Φ(b) T (−Kσ )Φ(b) = 1. The first of the derivak k ered which is not the case in this work. (18) is written dK0 (zi ) tives dzi is computed analytically as described before, alternatively in residual form as but the second term dKdzσ (zi i ) in (23) is more complicated ∂r du = −K0−1 (19) because of the implicit dependence of the state variables dzi ∂zi u, i.e., Kσ (zi , u(zi )). In this work an efficient analytical For the DMTO parameterization proposed in this work, adjoint method is introduced due to the many design varithe design domain is fixed. For this reason the deriva- ables in the DMTO approach. The adjoint method is ∂r tive ∂K∂z0 (zi i ) in the pseudo load vector ∂z involves only the based on the work presented in Rodrigues et al. (1995) i derivative of the assembled effective constitute element and Neves et al. (1995), but is nevertheless described here matrix Ee , which is determined analytically. However, for completeness. Applying the chain rule we have the DMTO parameterization introduces many design vari- dKσ (zi , u(zi )) ∂Kσ (zi , u) ∂Kσ (zi , u) du = + (24) ables, and it is thus more efficient to compute the displacedzi ∂zi ∂u dzi ment sensitivity using the adjoint method. Noting that the Again, the first term is the partial derivative of Kσ and this displacement uo can be expressed as uo = lT u, where l is term is computed on the element level in the same way as a vector with the value 1 at the DOF of interest, the sendescribed for the term dKdz0 (zi i ) . The second term of (24) insitivity of the displacement uo can be found analytically volving ∂Kσ /∂u is the difficult and costly part to compute as and still requires evaluation of state variable sensitivities duo T ∂r = −w (20) du/dzi for all design variables. However, note that we are dzi ∂zi not really interested in computing the term, but instead it where the vector w is the solution to the adjoint load prob- is to be pre- and post-multiplied with some eigenvectors in (23), i.e., lem T ∂Kσ (zi , u) du (b) K0 w = l (21) Φ(b) Φ = ... k ∂u dzi k (25) (b) T ∂Kσ (zi , u) (b) In this way, the factored stiffness matrix K0 is reused and −1 ∂r K Φ . . . − Φ 0 k k only a single forward/backward substitution is needed for ∂u ∂zi each displacement constraint uo before the displacement where the right hand side is arrived at by inserting the sensitivities in (20) are obtained analytically by vector expression for state sensitivities du/dz from (19) and rei multiplications. grouping terms exploiting symmetries. It is now conveThe direct approach to obtain the eigenfrequency sensi- nient to introduce the adjoint vectors v given as kk tivity is to differentiate (14) with respect to a design vari (b) T ∂Kσ (zi , u) (b) ( f ) T T (26) Φk K0−1 , make use of (14), and vkk = Φk able zi , premultiply by Φk ∂u noting that the system matrices are symmetric. Hence the Notice that vkk is the same for all design variables, and following expression is obtained for the eigenvalue sensithus only needs to be computed once for each iteration tivity in case of a simple, i.e., distinct, eigenvalue λ j , see of the optimization problem for each of the n(b) λ buckling e.g., Courant and Hilbert (1953) and Wittrick (1962). load factors included in the optimization problem (11). ! (f) ( f ) T dK0 When solving the linear systems of equations in (26) for dλk ( f ) dM (f) = Φk − λj Φk (22) the adjoint vector vkk , the factored stiffness matrix K0 can dzi dzi dzi be reused. The term ∂Kσ /∂u is derived analytically for Here it is assumed that the eigenvectors have been M- the ESL shell elements used, and by using (26) and (24) T orthonormalized such that Φ(kf ) MΦ(kf ) = 1. Again, the in (23) and regrouping terms, the buckling load factor seni) sitivity can be computed analytically as derivatives dKdz0 (zi i ) and d M(z dzi are computed analytically, as they involve only the derivative of the assembled effec- dλ(b) T dK0 (b) k tive constitute matrix Ee and the material candidate mass = Φ(b) Φ + ... k dzi dzi k (27) density ̺c with respect to zi . Note that in a finite element ! (b) T ∂Kσ (zi , u(zi )) ∂r (b) T implementation, all of these computations are performed . . . λ Φk − vkk Φk k ∂zi ∂zi on the element level, such that derivatives are only computed for elements depending on the given design variable In this way the sensitivities of the buckling load factors are computed very efficiently. The described DSA rezi . In a similar way the design sensitivity of a distinct quires full access to the finite element code used in order to implement analytical sensitivities of element mabuckling load factor is given as trices and vectors, and for implementation of the term ! (b) T dK0 dλ(b) (b) dKσ (b) k = Φk + λk (23) ∂Kσ /∂u needed for computing adjoint vectors in the anaΦk dzi dzi dzi lytical DSA of buckling load factors. 9 2.5 The SLP approach (30a) Φ(n) 0 Previous work by Sørensen and Lund (2013) concluded ρimin ,x jc ,yk that an SLP approach outperformed various Sequential max k = 1, 2, . . . , K (30b) s.t. Φ(n) k ≤ gk Quadratic Programming (SQP) approaches, primarily due to the nature of the manufacturing constraints to prevent (MC’s) (30c) intermediate void through the laminate thickness, i.e., MC4 from (10). As this work includes the same challenging manufacturing constraints, we rely on an SLP apρ(n) ∀i (30d) i ∈ ML proach once more, see for instance Arora (2004). The (n) x jc ∈ ML ∀ ( j, c) (30e) complexity of this work does, however, surpass that of Sørensen and Lund (2013) given the presence of several ∀k (30f) y(n) k ∈ [0, ∞[ non-linear structural constraints. Hence, in order to pose unconditionally feasible linearized programming prob- In (30d) and (30e), the set ML refers to the bounds of lems, we introduce an elastic programming technique the design variables which may change in each iteration due to the applied move limit strategy, described in the with merit functions. following subsection. Notice that feasibility of the linear manufacturing constraints can only be guaranteed if the initial linear problem is feasible, and if the move limits 2.5.1 Introduction of merit functions ML repeatedly include the previous design point. (n) (n) (n) (n) Merit functions ΦM = f (x jc , ρi , yk ), where the superscript (n) denotes the iteration number and M = 1 + K 2.5.2 Move limit strategy denotes an objective function and K non-linear structural Without precautions, any SLP approach is inherently subinequalities, are introduced to ensure feasibility of all linject to oscillating function and design variable values. earized optimization problems. Inspired by Svanberg’s Hence, a robust move limit strategy must be applied. In work on the Method of Moving Asymptotes (MMA), see this work, surveillance of a merit function is used to deem e.g., Svanberg (1987), we introduce the objective merit the validity range of the linearizations. An oscillating function merit function suggests that move limits should be reduced, whereas monotonous progress suggests expansion. ! K X 1 (n) 2 (n) (n) (n) Φ0 = m + a cyk + yk (28) In this work move limits are denoted δ and operate collec2 tively on all true variables such that k=1 (n) (n+1) max ρ(n) − δ, 0.0 ≤ ρ ≤ min ρ + δ, 1.0 ∀i (31) i i i (n) where m(n) = f (x(n) , ρ ) is the original objective funcjc i n and similarly for all x(n) (n) jc , but not the artificial variables yk tion, x(n) and ρ are the true optimization variables, while jc i where the initial bounds are maintained throughout to eny(n) k ∈ [0.0, ∞[ are artificial optimization variables, also sure LP feasibility. Rather than the objective merit funcknown as slack variables, that are subtracted the struc- tion (28), we monitor the oscillation merit function (32). (n) (n) tural non-linear inequality constraints g(n) (n) k = f (x jc , ρi ), (n) max Φ(n) ∀k (32) resulting in the constraint merit functions osc = Φ0 1 + max gk − gk , 0.0 Contrary to (28), the merit function (32) maintains a direct (29) measure of infeasibility even for all y(n) = 0.0 which is k found more efficient by experience. Let O(n) denote the that in combination with (28) ensure feasibility of the oscillation indicator for iteration (n) such that (n−1) non-linear structural constraints. In (28), c is a positive Φ(n) osc − Φosc (n) (33) penalization constant ensuring that the artificial variables O = (n−2) Φosc − Φ(n−1) osc become expensive when larger than the desired zero y(n) k values. In agreement with the practical considerations and Pseudo code for reduction or expansion of the move limits recommendations in Svanberg (2004), all non-linear con- δ, depending on the oscillation indicator, appears in Fig. straints are normalized with respect to gmax k , c is initially 3. set to 100.0, and the constant a is set to m(1) , serving the In the pseudo code shown in Fig. 3, α ∈ [0.0, 1.0[ is the purpose of proper scaling between the objective function move limit reduction factor, β ≥ 1.0 is the move limit exand the non-linear constraints. With the introduction of pansion or recovery factor, and OscCheck prevents mod(28) and (29), the optimization problem which is to be lin- ification of move limits immediately upon reduction for earized and solved sequentially in a number of iterations stabilization, initialized to OscCheck = −1. In this work, α = 0.5 and β = 4.0 are found appropriate. by an efficient LP optimizer is now defined as (n) (n) max , k = 1, 2, . . . , K Φ(n) k = gk − yk ≤ gk 10 if (OscCheck > 0) then (n) if O < 0.0 then δ = δα OscCheck = 0 else 1 δ = min δα− β , δini end if else OscCheck = OscCheck + 1 end if In case of satisfactory CC’s, whether or not to proceed to the next continuation step, if any, depends on the obtained level of discreteness of the design variables. To this end we introduce two slightly modified measures of non-discreteness compared to those applied in Sørensen and Lund (2013), taking into account e.g., different sizes of the sub-domains, Ωdl . The measures Mdnd and Mcnd denote the density (ρi ) and candidate (x jc ) nondiscreteness, respectively. P 4 d,l Vdl ρi (1 − ρi ) (n) P · 100% (38a) Mdnd = d,l Vdl Figure 3: Pseudo code for controlling the reduction or 2 P 1−x jc 2 Qnc expansion of the move limits δ V ρ d,l dl i c=1 1− 1c (n) n P · 100% (38b) = Mcnd d,l Vdl ρi 2.5.3 Continuation strategy Most places in (38) and the following, the iteration suExperience has shown it efficient to increase the penal- perscript (n) is omitted for clarity. Proper association ization power p in a stepwise manner, known as a con- between indices dl, i, and j, as exemplified in (6), is a tinuation approach. Instead of starting out from the seem- prerequisite for both measures. The measure of density ingly obvious and classical case without penalization, i.e., non-discreteness M is normalized to yield 0.0% in case dnd from p = 0.0, it is noticed that the bi-linear product be- ρ ∈ {0, 1} ∀i and 100.0% in case ρ = 0.5 ∀i. The meai i tween the variables ρi and x jc in (5) is unconditionally sure of candidate non-discreteness M is linearly depencnd non-convex. An extensive parameter study has revealed it dent upon the appurtenant values of ρ such that it yields i to be efficient to start out from a limited but still notice- 100.0% for x = 1 ∀( j, c) if ρ = 1.0 ∀i and 50.0% if c i jc able penalization level. The parameter study has shown ρ = 0.5 ∀i, and son on. The M measure yields 0.0% i cnd the sequence in case x jc ∈ {0, 1} ∀( j, c) independent of ρi , or in case ρ p = {1.0, 2.0, 4.0} (34) i = 0.0 ∀i independent of x jc . This linear ρi dependence is fair in that a distinct candidate selection is insignificant to be robust for all considered cases. Notice that the se- for vanishing topology variables. Continuation to the next quence (34) is allowed to finish prematurely in case of penalization step, if any, is found relevant only in case (n) achieving a satisfactory feasible, near 0/1 design before (n) , Mcnd Mnd = max Mdnd > ǫ0/1 (39) the last step. This is elaborated in Section 2.5.4. Pseudo code for the convergence requirements appears in 2.5.4 Convergence requirements Fig. 4. if (CC1 < ǫΦ ) then if CC2 < ǫy then if CC3 < ǫg then if (p < pmax .and. Mnd > ǫ0/1 ) then Increase penalization power p δ = δini OscCheck = −1 else Convergence end if end if else Restart optimization c = 10.0c end if end if A continuation step is converged when fulfilling three Convergence Criteria (CC): At first, we require a sufficiently small change in the merit function (28) (CC1). This has been established to indicate if the optimization procedure has converged to a minimum. Secondly, we require vanishing artificial variables (CC2), and thirdly, we require an acceptable level of feasibility (CC3). The procedure is outlined in the following. Ultimately, fulfilment comes down to comparison with appurtenant tolerances, denoted ǫ. A sufficiently small, absolute change in the merit function (28) is defined as (n) Φ0 − Φ(n−1) 0 < ǫΦ (CC1) (35) (n−1) Φ0 Vanishing artificial variables are defined as y(n) < ǫy ∀k (CC2) k ∞ Lastly, acceptable feasibility is defined as g(n) − gmax < ǫg ∀k (CC3) k k ∞ (36) Figure 4: Pseudo code detailing the convergence requirements (37) It is seen in Fig. 4, that in case (CC1 < ǫΦ ) but (CC2 > ǫy ), it appears that the current penalization constant c was 11 insufficient to ensure near zero valued artificial variables. As Svanberg (2004) suggests, c is increased, here by a factor 10.0, and the optimization problem is restarted. In case the convergence requirements on ǫΦ and ǫy are met, it comes down to the requirement on ǫg whether additional iterations and move limit modifications are required to facilitate final convergence. Otherwise, a new continuation step, if any, with increased penalization power p is initiated, however, only in case of an unacceptable level of non-discreteness, governed by Mnd . In case of continuation with increased p, the optimization problem at hand has changed for which reason move limits δ and the counter OscCheck are consistently relaxed to accommodate this new problem. Experience has shown that ǫΦ = ǫg = 10−3 , ǫy = 10−4 , and ǫ0/1 = 0.1% entail an acceptable tradeoff between the required number of iterations and feasibility and discreteness of the results. Results to follow are computed by use of our in-house finite element and optimization framework, the so-called MUltidisciplinary Synthesis Tool (MUST), see MUST (2013), which is compiled using Intel Visual Fortran together with the Intel MKL library. In order to cope with the large number of linear constraint equations stemming from the candidate material formulation (3) and the manufacturing constraints (7), (8), and (9), version 7.2-9 of the Sparse Nonlinear OPTimizer (SNOPT) by Gill et al. (2005) is applied. For all results to follow, SNOPT has been configured with default settings to solve the mathematical programming problem (30) through the presented SLP approach. 2.6 Simple 0/1 rounding The considered optimization problem (11) is challenging to drive to completely binary design variables with the suggested density approach. This is primarily because of structural sensitivities of both operational signs, but likewise due to the difficult manufacturing constraints. In this work, we apply simple rounding of the design variables to finalize the obtained results into truly discrete designs, and leave for instance advanced finalization techniques, or explicit penalization of intermediate designs to future work. Let ρ∗i denote the topology variable value after simple rounding, defined as ρ∗i 1 = 0 if ρi ≥ 0.5 else 1 = 0 for (40) Let x∗jc denote the candidate variable values after simple rounding, defined such that only the originally dominating candidate c is rounded up for all candidate domains j, given as x∗jc else n o max x j1 , x j2 , . . . , x j(nc ) (41) Notice that such simple rounding does not guarantee feasibility nor optimality of the posed optimization problem (11), see Nemhauser and Wolsey (1988). However, as results in Section 4 will demonstrate, obtained measures of non-discreteness Mnd are mostly near-zero, thereby indicating only minor perturbations upon rounding. The effect of the suggested simple rounding appears in Section 4 and is discussed further in Section 5. 3 Numerical examples This section introduces several numerical optimization problems concerning a finite element model of a generic main spar used in many designs of wind turbine blades. The parameterization into candidate and geometry domains, directly associated with the design variable distribution, is however unique for all problems, i.e., Steps 1-2 are identical, but Steps 3-4 differ for all problems, see Fig. 1. 3.1 The finite element model The geometry of the main spar is identical to the one applied in Lindgaard and Lund (2010) where fiber orientations were optimized with respect to buckling load factors applying geometric non-linear analysis. The considered main spar is truncated to a length of 14.0m and has an inner diameter of 0.88m at the fixed root section. The finite element model of the main spar appears in Fig. 5 and consists of 1,792 degenerated 9-node ESL shell elements with five DOF’s per node, resulting in a total of 36,160 DOF’s. See e.g., Ahmad et al. (1970) or Panda and Natarajan (1981) for element details. All ESL shell elements represent 20 layers, each with a uniform thickness. A ply thickness of 2.5mm has been selected as a tradeoff between the number of design variables and the total thickness required in order to have a realistic load case. The finite element mesh discretization of Fig. 5 has been checked for convergence as follows: Modeling the main spar entirely with 0◦ plies oriented along the global z-axis (m = 2752.27kg), the mesh was refined until stable values of the tip displacement (utip = 0.5846m) and the lowest buckling load factor (λ1(b) = 8.810) and eigenfrequency (ω1 = 4.378 · 2π rad s ) were obtained. The main spar is modeled with clamped boundary conditions at the circular end of the root section and the applied tip load resembles the most critical load case for the wind turbine blade, a so-called 50 year gust scenario, subjecting the blade to a case of extreme flap-wise bending. The load is introduced as a uniform pressure, illustrated by the hatched rectangle at the tip in Fig. 5. The distributed load has an intensity of q= 12 164.7kN = 559kPa 0.3m · 1m (42) x jc , ρi 0m t) oo (R 3m ) id (M Figure 7: The longitudinally coinciding candidate and geometry domain parameterization is referred to as the Long-Long parameterization m 12 y z 4m )1 ip (T x z Figure 5: Finite element model of a generic main spar, clamped at the circular end of the root section and tapered towards the tip that is subjected to a uniform pressure load at the hatched rectangular area. Cross sections of the root and the tip appear in Fig. 6. All ESL shell elements have their first principal material direction aligned with the global z-axis, and their surface normals pointing outwards. At the tip, the node marked by the bottom dot is subjected to a displacement constraint The structural setup resembles testing of wind turbine blades in a controlled environment, see Overgaard et al. (2010). Neither the geometry of the main spar nor the applied load case introduce torsion into the model. Geometric linear analysis is used throughout this paper to limit the computational time. The proposed method does, however, allow for the use of geometric non-linear analysis, and the authors recognize the limitations associated with linear analyses. This is further discussed in Section 5.1. Lindgaard and Lund (2010) showed that geometric linear analysis generally overestimates the critical load in buckling load optimization. 3.2 Parameterization of the generic main spar Parameterization of the finite element model is an important step in the optimization procedure as structural performance and manufacturability of the optimized designs depend hereupon. The production method for the presented main spar relies on the application of a mandrel that essentially dictates the inner shape of the main spar. The root of the mandrel is bolted to a rigid wall and the mandrel is then covered by mats or blocks of different materials and principally “built up” from the inside in a series of steps. First, GFRP biax fiber mats are typically wrapped around the full length of the mandrel. Next, full-length GFRP UD fiber mats are rolled along the top and bottom surfaces of the mandrel. On the sides/webs of the mandrel, blocks of lightweight foam or balsa material are positioned. These steps are systematically repeated, resulting in a structure with varying thickness at different locations around the mandrel. Finally, the composite structure is cured and the finished main spar can be pulled off the mandrel. With this production method in mind, an obvious question crops up, namely where to most appropriately allocate the available material candidates, to obtain a high-performance, manufacturable structure? The design freedom, but hence also the potential level of structural complexity, is directly linked to the parameterization into geometry and candidate domains, see Fig. 1. If, for instance, the manufacturer is accustomed to apply large rolls of fibrous material with a width of 1.0m, then the parameterization into geometry and candidate domains should accommodate just this. In this work, we compare the optimization outcomes on basis of nine representative candidate and geometry parameterizations of the generic main spar. This is done to give insight into the relation between potential weight saving and complexity, subject to identical structural criteria and manufacturing constraints. The constraint specifications are elaborated in Section 3.2.2. The finite element mesh discretization of Fig. 5 (Step 1 in Fig. 1) is deemed too fine for the arrangement into sub-domains Ωdl (Step 2 in Fig. 1). The arrangement of the main spar mesh into sub-domains appears in Fig. 6 that illustrates the main spar, cut along the longitudinal direction of the upper surface (the dotted lines) and unfolded as a flat surface. The main spar mesh is arranged into a total of 28 × 8 = 224 sub-domains, identical for all layers. The sub-domains are equally spaced longitudinally. Circumferentially, the sub-domains vary in width, see the bold line markings to the left and right of Fig. 6. Concerning Steps 3-4 in Fig. 1, i.e., the parameterization into geometry domains and candidate domains, associated with variables x jc and ρi , respectively, the following nine parameterizations are considered. The nine parameterizations are constructed on basis of Fig. 7 and Fig. 8, where the sub-domains are parameterized into coinciding candidate and geometry domains longitudinally and circumferentially, respectively. Figure 7 represents 13 Ωdl (Tip) (Root) Figure 6: Left: Cross sectional view of the circular root section. Bold lines denote eight circumferential design domain arrangements. Mid: Unfolded surface view of the main spar, cut along the longitudinal direction of the upper surface. The cut is illustrated by the dotted lines. The generic main spar mesh is arranged into 28 × 8 = 224 sub-domains, Ωdl . Right: Cross sectional view of the tip section x jc , ρi Table 1: The nine considered parameterizations into candidate domains, x jc , and geometry domains, ρi Candidate domains (x jc ) Long Long Long Circ Circ Circ Grid Grid Grid Figure 8: The circumferentially coinciding candidate and geometry domain parameterization is referred to as the Circ-Circ parameterization a parameterization where both the candidate domains x jc and the geometry domains ρi coincide longitudinally. For this reason we denote this parameterization Long-Long for candidate domains, x jc , and geometry domains, ρi , respectively. Similarly, Fig. 8 represents the so-called CircCirc parameterization with circumferentially coinciding candidate domains, x jc , and geometry domains, ρi , respectively. These particular parameterizations represent a relatively low level of complexity, i.e., a high degree of manufacturability. For this reason, exactly these two parameterizations are considered in detail in the following sections. The low level of complexity associated with these particular parameterizations is in contrast to the socalled Grid-Grid parameterization, where candidate and geometry domains coincide with the sub-domain arrangement in Fig. 6. This parameterization is hence considered quite complex and difficult to manufacture. Allowing candidate and geometry domains to be non-coinciding within the three described parameterization types, i.e., the longitudinal (Long), the circumferential (Circ), and the grid type (Grid) parameterizations, a total of nine uniquely defined candidate-geometry domain parameterizations can be defined, see Table 1. These nine parameterizations into candidate domains, x jc , and geometry domains, ρi , give insight into the relation between potential weight saving and complexity. Geometry domains (ρi ) - Long Circ Grid Long Circ Grid Long Circ Grid Table 2: Properties of the considered candidates Property E11 E22 E33 G12 G23 G13 ν12 ̺ 3.2.1 Units [GPa] [GPa] [GPa] [GPa] [GPa] [GPa] [kg/m3 ] UD 34.00 8.20 8.20 4.50 4.00 4.50 0.29 1910.00 Biax 16.50 16.50 8.20 9.50 4.00 4.50 0.29 1910.00 Foam 0.16 0.45 130.00 Candidate materials The numerical examples include six different candidate materials commonly applied in the wind turbine industry, i.e., nc = 6. Candidates one to four represent GFRP UD plies with {−45◦ , 0◦ , 45◦ , 90◦ } fiber orientations. The 5th candidate represents a GRFP {±45◦ } biax ply with properties obtained on basis of the {−45◦ , 45◦ } UD data. The 6th and last candidate represents a lightweight isotropic foam material such that a sandwich structure is a possible outcome of the optimization problem. Candidate properties appear in Table 2. The void material, E0 from (5), 14 sible without candidate preference, found efficient by exTable 3: Settings concerning structural criteria and manperience. This implies an initial mass m = 2324.78kg ufacturing constraints or m = m = 2752.27kg, including or excluding foam as a candidate, respectively, where m denotes the maximum q attainable mass. The potential to obtain a feasible solution λ(b) ω = λ( f ) u n(b) n(λf ) S CL T λ with an end mass lower than m is clear from a comparison 3.0 2π rad 1.0m 10 10 2 8 0.10 with the presented values from modeling the main spar s entirely with 0◦ plies oriented along the global z-axis, see Section 3.1. Move limits are initialized as δini = 0.20. The is modeled as a weightless isotropic material with one move limit range 0.0 ≤ δ ≤ δini is adaptively modified as millionth the stiffness of the GFRP UD candidate, i.e., prescribed in Section 2.5. E11 = 34kPa, and identical Poisson’s ratio. Because other industries do not allow sandwich designs, results for the nine parameterizations in Table 1 will also be listed without foam as a candidate, in which case nc = 5. Conse- 4 Results quently, the considered number of design variables varies between 953 for the Long-Long parameterization without Tables 4-5 provide detailed result overviews of the DMTO foam to 31,137 for the Grid-Grid parameterization includ- approach of the nine different parameterizations introing foam. Notice that for all parameterizations, the entire duced in Section 3, both with and without foam as a caninnermost layer of the generic main spar is modeled as a didate. Table 4 presents the original, non-rounded results single, unity valued topology variable to eliminate the risk on basis of the SLP approach presented in Section 2.5. of holes through the thickness. A star ∗ in front of the total number of iterations #It. indicates that the SLP approach has been restarted once with up-scaled c value to obtain vanishing artificial vari3.2.2 Constraint specifications and initial settings ables, yk . Table 5 presents the results upon finalization In agreement with the main spar study in Overgaard et al. by the simple rounding described in Section 2.6. The (2010), the representative bounds listed in Table 3 have results in Table 4 and Table 5 are referred to as origibeen chosen for the structural constraints in (11b)-(11d). nal and rounded results, respectively. For easy comparIn order to cope with potentially shifting eigenvalues, we ison, Fig. 9 provides a graphical overview of the original consider the first ten buckling load factors and eigenfre- DMTO results of the nine parameterizations with foam. quencies, assumed ordered by magnitude. The displace- In the figure, measures of non-discreteness, Mnd from ment constraint limits the global y-displacement of the (39), above 1.0% have been truncated. See Table 4 for bottom tip node, marked in Fig. 5, preventing collision details. As mentioned previously in Section 3.2, rounded between blade and tower. With respect to the manufac- results of the Long-Long and Circ-Circ parameterizations turing constraints (11e), see Section 2.3 for details, we with and without foam, respectively, are picked out for apply the limit values apparent rightmost in Table 3. A detailed representations given their limited complexity. thickness variation rate of ±2 plies (S = 2) between adja- Apart from demonstrating the versatility and robustness cent geometry domains, ρi , is used to ensure sufficiently of the DMTO method, results from the additional paramesmooth external ply drop transitions for all parameteri- terizations primarily serve a comparative purpose in order zations of the generic main spar. For the particular main to assess the relation between potential weight saving and spar example considered in this work, we apply a contigu- complexity for the considered main spar example. Figure ity limit as large as eight identical plies through the thick- 10 illustrates an exploded view of the allocation of canness (CL = 8), being considerably more than the com- didates for the Long-Long parameterization with foam, monly applied limit of four, see e.g., Le Riche and Haftka seen from the fixed root end. Candidate allocation is iden(1993) or Toropov et al. (2005). Nevertheless, the wind tical longitudinally. Notice that the allocation among the turbine industry is less restrictive than the aerospace in- candidates depicted to the right of Fig. 10 is given with ′ dustry; hence larger amounts of identical UD plies can be respect to a local coordinate axis, denoted y . Figure 11 ilaccepted. The influence of the applied contiguity limit is lustrates the allocation of candidates for the Circ-Circ pafurther scrutinized in the discussion of the results. These rameterization without foam where bottom and top illussettings imply that the number of MC’s vary between trate the inner and outer surfaces, respectively. Candidate 1,144 for the Long-Long parameterization without foam allocation is identical circumferentially. Figure 12 shows to 20,800 for the Grid-Grid parameterization including the design iteration history for the Long-Long parame(b) foam with 21,584 and 182,016 non-zero coefficient ma- terization with foam, illustrating the evolution of m, λ1 , trix entries, respectively. The design variables are initial- λ(1f ) , |uo |, Mcnd , Mdnd , kyk k∞ , kgk − gmax k k∞ , and ∆(x jc , ρi ); ized as x jc = n1c for all candidate variables and ρi = 1.0 see the caption for further explanations and normalization for all topology variables to start out as feasible as pos- details. 15 Table 4: Tabular overview of the original DMTO results of all parameterizations, both with and without foam as a candidate. #It. denotes the total number of iterations. A star ∗ in front of #It. denotes that the SLP approach has been restarted once with up-scaled c value Parameterization With foam Without foam (x jc − ρi ) m [kg] λ(b) 1 λ(b) (f) λ1 λ( f ) |u| u Mcnd /Mdnd [%] #It. m [kg] λ(b) 1 λ(b) (f) λ1 λ( f ) |u| u Mcnd /Mdnd [%] #It. Long-Long Long-Circ Long-Grid 1249 1.000 2.969 1.000 1240 1.037 2.938 1.000 1225 1.000 2.926 1.000 0.282 / 0.672 41 0.062 / 0.000 28 0.159 / 0.999 40 1802 1.000 4.218 1.000 1841 1.081 4.328 0.999 1807 1.118 4.378 1.000 0.000 / 3.079 49 0.001 / 0.451 44 0.000 / 1.728 *142 Circ-Long Circ-Circ Circ-Grid 1431 0.999 5.008 1.000 1519 1.001 4.690 0.999 1428 1.000 5.019 1.000 0.180 / 0.000 41 0.316 / 0.305 *91 0.139 / 1.518 57 1850 1.117 4.178 1.000 1854 1.069 4.334 1.001 1746 1.014 4.466 1.000 0.815 / 0.273 0.829 / 0.971 0.559 / 2.177 39 44 54 Grid-Long Grid-Circ Grid-Grid 1171 0.999 2.738 1.000 1181 0.999 2.787 1.000 1163 0.999 2.789 1.000 0.671 / 0.120 63 0.947 / 0.196 84 1.053 / 1.408 81 1818 1.148 4.205 0.999 1848 1.095 4.252 1.001 1734 1.000 4.455 1.000 3.517 / 0.984 2.715 / 0.337 1.619 / 1.446 48 44 64 Table 5: Tabular overview of the rounded DMTO results of all parameterizations, both with and without foam as a candidate Parameterization With foam Without foam λ(b) 1 λ(b) (f) λ1 λ( f ) |u| u # Violated MC’s Long-Long Long-Circ Long-Grid 1246 0.930 2.961 0.995 1242 1.081 2.951 0.999 1221 0.970 2.950 1.001 Circ-Long Circ-Circ Circ-Grid Grid-Long Grid-Circ Grid-Grid (x jc − ρi ) 5 λ(b) 1 λ(b) (f) λ1 λ( f ) |u| u # Violated MC’s 0 0 0 1832 1.138 4.282 0.953 1837 1.081 4.358 0.998 1805 1.143 4.396 0.994 0 0 0 1431 0.964 5.006 0.999 1520 0.970 4.656 0.994 1429 0.935 5.054 0.994 0 0 0 1848 1.121 4.180 1.001 1844 1.069 4.378 1.003 1734 1.017 4.477 1.003 0 0 0 1159 0.887 2.738 1.001 1159 0.873 2.804 1.004 1140 0.807 2.776 1.002 0 0 0 1832 1.185 4.249 0.967 1846 1.101 4.280 0.994 1733 1.028 4.478 0.995 29 41 0 m [kg] Discussion The discussion of the results is done in the following steps. Initially, some general comments about the original non-rounded results are stated. Secondly, the overall effects of rounding are discussed. Thirdly, we discuss the results of the Long-Long and Circ-Circ parameterizations, respectively, with and without foam in detail. Finally, general comments about the performance of the DMTO method are stated. 5.1 Original result tendencies It is clear from the results of Table 4 and Fig. 9 that parameterizations with foam as a candidate significantly outperform those without foam. The optimizer recognizes the foam candidate as a profitable means of obtaining high moments of inertia, beneficial for the considered m [kg] flap-wise bending load case. With foam, the end mass ranges from 0.42m ≤ m ≤ 0.55m as opposed to a range from 0.63m ≤ m ≤ 0.67m without foam. The lowest mass is 1163kg for the original Grid-Grid parameterization with foam, and the largest being 1854kg for the original Circ-Circ parameterization without foam. It is not surprising that the Grid-Grid parameterization with foam yields the lowest mass as this parameterization reflects ultimate design freedom, supporting rapid changes in both geometry and candidate preference. Hence, the Grid-Grid result with foam should be the natural choice for a highperformance design; that is if manufacture is possible, which is doubtful due to the high degree of complexity. The displacement constraint is active for all parameterizations. Most parameterizations do likewise end up with active constraints on buckling load factors, whereas the constraints on eigenfrequencies are inactive throughout as a consequence of low mass and high stiffness. Neverthe- 16 1 m/m Mnd [%] # Iterations / 100 0.8 0.6 0.4 0.2 0 Long−Long Long−Circ Long−Grid Circ−Long Circ−Circ* Circ−Grid Grid−Long Grid−Circ Grid−Grid Figure 9: Graphical result overview of the original DMTO results of the 9 parameterizations with foam. The star marking at Circ-Circ∗ denotes that the SLP approach has been restarted once with up-scaled c value. Mnd measures are truncated at 1.0%, see Table 4 for details 4 analysis comparison revealed that the linear predictions are up to 17% larger for parameterizations without foam, and 10% larger for parameterizations with foam. In spite of these deviations, we maintain linear analyses to reduce the computational time. It is, however, stressed that the DMTO method supports non-linear analyses as well. 3.5 Normalized Values 3 m (b) λ1 2.5 (f) λ1 |uo | Mcnd (xjc ) 2 Mdnd (ρi ) kyk k∞ 1.5 kgk − gkmax k∞ ∆ (xjc , ρi ) 1 0.5 0 1 5 10 15 21+ 25 Iteration No. 30 35 38+ 41 In section 2.4, we state that including nλ(b) buckling load factors takes care of crossing eigenvalues (mode switching) during the optimization process. In all the numerical examples, the ten lowest buckling load factors were thus included as constraints in the optimization problem. To check if including the ten lowest values has sufficed, the final ten buckling load factors have been analyzed for all numerical examples. Here it has been found that the difference in magnitude between the first and the 10th value is on average 17% and 28% for the parameterizations with and without foam, respectively. The possibility for the 11th load factor changing more than 17% or 28% between two successive iterations is believed to be negligible; hence including the ten lowest positive buckling load factors has been adequate for controlling mode switching for the applied numerical examples. Figure 12: Design iteration history for the Long-Long parameterization with foam. The mass m is normalized with respect to the initial mass. The structural perfor(f) mance constraints λ(b) 1 , λ1 , and |uo | are normalized with respect to their bounds, see Table 3. The measures of nondiscreteness, Mcnd and Mdnd , appear as decimal numbers. The values of the largest artificial variable, kyk k∞ , and the largest infeasibility among the structural constraints, kgk − gmax k k∞ , are shown in accordance with (36) and (37), respectfully. ∆(x jc , ρi ) is the Euclidean norm of the change in design variables between two successive iterThe measures of non-discreteness, Mcnd and Mdnd from ations. A change in penalization is indicated with a ”+” (38), are generally largest for the Grid-Long, Grid-Circ, sign next to the iteration number in which the penalization and the Grid-Grid parameterizations without foam. The was increased reason for this may be that this particular group of parameterizations represents the most challenging optimization less, one can only ensure demands on structural criteria problems, considering the number of design variables, the when present in the optimization problem. number of constraints, and the fact that those parameteriAs highlighted in Section 3.1, the numerical examples zations without foam call for a larger extent of thickness have been conducted using geometric linear finite element variation than parameterizations with foam where sandanalysis. In order to estimate the effects of the geometric wich structures are natural outcomes. Experience has non-linearity on the active constraints, a geometric non- shown that neither increasing penalization nor different linear analysis of the two initial designs for the param- continuation approaches improve the obtained levels of eterizations with and without foam as a material candi- non-discreteness. One way of addressing this issue could date, see Section 3.2.2, has been conducted. These analy- be to use explicit penalization of intermediate valued deses show that the linear tip displacement is within 5% of sign variables as suggested in e.g., Hvejsel et al. (2011) the geometric non-linear tip displacement. The buckling or Kennedy and Martins (2013). Modification or even re17 y′ replacements y′ y′ y′ −45◦ (UD) y′ [8] [1] y [7] x z 0◦ (UD) [2] y′ [3] ±45◦ (Biax) Foam (Iso) [4] [6] +45◦ (UD) 90◦ (UD) [5] Void y′ y′ y′ Figure 10: Rounded DMTO result of the Long-Long parameterization with foam. The Long-Long parameterization implies that candidate allocations and thicknesses of the eight longitudinal design domains, marked by [1]-[8], are identical from the root to the tip of the main spar moval of the troublesome constraints that prevent intermediate void (MC4), see (9), is likewise considered attractive as it may facilitate application of highly robust SQP or interior point optimizers, see Sørensen and Lund (2013) for further discussion on this issue. The obtained levels of non-discreteness are all less than 4% which is found acceptable. Robust solutions for obtaining even more discrete results at this stage, i.e., prior to the following finalization by rounding, are left for future work. Notice that the Long-Circ parameterization with foam converges before the last continuation step as a result of a sufficiently near-zero measure of non-discreteness, Mnd , see (39). The total number of iterations ranges from 28-142 with an average of 59. The star ∗ in front of the two parameterizations in Table 4; Circ-Circ and Long-Grid, with and without foam, respectively, denotes that these particular parameterizations were restarted once with up-scaled c values to obtain vanishing artificial variables, yk . Experience has shown that the initial value c = 100.0 yields better results than c = 1000.0 or more for which reason up-scaling is only applied if necessary in agreement with Svanberg (2004). 18 to 22. The DSA time of the Grid-Grid parameterization with foam exceeds that of the Long-Long parameterization with foam by 22%. Given that these two parameterizations involve 31,137 and 953 design variables, respectively, clearly demonstrates the efficiency of the adjoint formulation when having many design variables. The three-step continuation sequence (34) is found to yield better results than applying a single, constant penalization value throughout. Likewise, the sequence is found more robust than additional continuation steps or even starting out from lower values of p. Too many continuation steps impose a risk of getting stuck at an intermediate design point with no chance of getting rid of the artificial design variables. 5.2 Rounded result tendencies Results upon finalization by the simple rounding described in Section 2.6 appear in Table 5. The effect of rounding on the original mass varies between -23kg for the Grid-Grid parameterization with foam to +30kg for the Long-Long parameterization without foam. Changes in the original mass are generally reflected upon changes in the criteria functions. Rounding generally affects the The sequential time consumption associated with DSA parameterizations with foam as a candidate significantly exceeds the evaluation of structural criteria by a factor of more than those without. This is due to the large differ18 (Outer surface) −45◦ (UD) 0◦ (UD) +45◦ (UD) 90◦ (UD) ±45◦ (Biax) Void 0.05m (Root) 0.0m (Tip) (Mid) 3.0m 12.0m x 14.0m Figure 11: Rounded DMTO result of the Circ-Circ parameterization without foam. The Circ-Circ parameterization implies that the candidates are distributed in 0.5m wide circular belts, wrapped around the entire circumference of the main spar, resulting in 28 unique candidate belts throughout the length ence in the constitutive properties, see Table 2. The buckling criterion is particularly affected, being more locally dependent upon change than e.g., the tip displacement constraint. Rounding of the Grid-Grid parameterization with foam yields a buckling load factor constraint violation of 19.3%. On average, however, rounding causes structural criteria constraint perturbations < 3%. Rounding of the two parameterizations; Grid-Long and Grid-Grid, both without foam, causes 29 and 41 violations of the manufacturing constraints, respectively. The violations are in both cases associated solely with the constraints on contiguity (MC3), see Section 2.3.3, allowing at most 8 identical contiguous candidates throughout the 20 layers of the 224 candidate domains. Upon rounding, more than 8 GFRP UD plies oriented at 0◦ appear contiguously. As previously mentioned, infeasible constraints are a possible risk associated with this simple rounding scheme due to the decoupling of the optimizer. Nevertheless, it is stressed once more that DMTO results should not be viewed as final designs, ready to manufacture, but rather as a vital source of inspiration for thickness variation and stacking sequences throughout the entire structure. 5.2.1 Long-Long with foam The rounded DMTO result of the Long-Long parameterization with foam appears in Fig. 10. Candidate allocation and domain thicknesses are inherently identical longitudinally, hence not allowing a tapered geometry towards the tip. Despite these inherent restrictions, the allocation of candidates agrees quite nicely with existing designs. The moment of inertia Ixx is large in order to cope with the displacement constrained, flap-wise bending load case. This is clear from the predominant stacking of 0◦ GFRP UD plies at the top and bottom domains, denoted by numbers [1] and [5] in Fig. 10, respectively. 0◦ GFRP UD plies likewise appear at the outermost active layers around [2], [4], [6], and [8]. These plies contribute to Ixx as well. The two sides [3] and [7] are free from material at the outermost two layers and otherwise predominantly constituted by the lightweight foam candidate. The bottom domain [5] contains more 0◦ GFRP UD plies than the top domain [1], probably to resist the first buckling loads, dominant along the bottom pressure side [5]. Notice the presence of at most eight contiguous UD plies, thereby satisfying the imposed contiguity limit (MC3). In spite of feasibility, it is, however, recognized that having too thick regions with identical fiber orientation is typically unwanted; especially in the more conservative aerospace industry. Tightening the contiguity limit to the commonly applied value of four has been tested to result in additional foam plies in between the thick stacks of 0◦ GFRP UD plies. Not surprisingly, a tighter contiguity limit increases the final mass. From a manufacturing point of view, rapid encapsulation of just a few plies of foam in between fibrous layers such as occurring in [5], is undesirable. Multiple encapsulations are nevertheless a perfectly feasible outcome with the current DMTO formulation, and future work should impose the aforementioned sandwich constraints, forcing foam plies to be grouped together through the thickness of the candidate domains. Such constraints should likewise ensure the block of foam to be enclosed by fibrous material from both sides, unlike the regions [3] and [4]. Manufacturing constraints ensuring minimum proportions or presence of all material candidates as well as constraints limiting the change in fiber orientation between adjacent in-plane candidate domains could likewise be considered, but are, however, left for future extensions of the DMTO method. Notice that the design is not entirely symmetric along the xz and yz coordinate planes. This not entirely symmetric design across the vertical yz plane may be a beneficial way to exploit elastic couplings, obscure at first glance. Another explanation may be that the optimizer has settled on a sub-optimal minimum. Furthermore, due to the flap-wise bending load case, the solution does not con- 19 tain more than three GFRP plies with other orientations than 0◦ in total. Had the examples been formulated with an additional torsion load case, other fiber orientations would probably occur in greater numbers. Nevertheless, the rounded result appears to provide a sound offset for detailed post-processing. Figure 12 shows a typical iteration history graph; here for the Long-Long parameterization with foam. At the initial design point, the displacement constraint is infeasible, and the optimizer initially focuses on obtaining a feasible design at the expense of an increase in mass. Feasibility is obtained in iteration number four; showing that the merit function approach effectively copes with infeasibilities. The candidate non-discreteness is rapidly decreasing in pace with the optimizer recognizing that UD material should be allocated on the top and bottom faces of the main spar to achieve feasibility. The measure of density non-discreteness reaches its maximum value of 3.6% in the 6th iteration and drops to a stable value around 1% at the 12th iteration. At the 7th iteration, the buckling constraint becomes infeasible and remains so until iteration number 11. However, it oscillates around the feasibility limit until it becomes active at iteration number 21 which then satisfies convergence criteria CC3, causing an increase in penalization. Notice that during this phase, the change in the design variables decreases for each iteration; showing that the move-limit strategy indeed responds to oscillating constraints. Up until the first increase in penalization, the mass has decreased by 41.6% with respect to the initial mass. After this change in penalization both the displacement and buckling constraints become infeasible until activity is obtained in iteration number 29. From this iteration until the next increase in penalization, the candidate non-discreteness decreases from 5.2% to 0.26%, and the mass decreases as well until CC1 is finally satisfied. From iteration 38 to 41, the mass is increased from 1247kg to 1249kg. However, the measure of density non-discreteness is reduced from 1.1% to 0.67%. Final convergence is facilitated by satisfying CC2 and CC3 in iteration number 40 followed by CC1 in 41. Overall, the presented iteration history demonstrates that the SLP approach with merit functions is quite efficient at obtaining a feasible and near discrete design in spite of great non-linearity of the involved structural criteria. 5.2.2 Circ-Circ without foam The rounded DMTO result of the Circ-Circ parameterization without foam as a candidate appears in Fig. 11. Generally, the combination of the flap-wise bending load case together with the displacement constraint calls for a high moment of inertia Ixx and hence predominantly 0◦ GFRP UD plies on the top and bottom faces. This is also clear from the results of the Long-Long parameterization. For the Circ-Circ parameterization the candidate domains are grouped together in circular belts around the circum- ference of the main spar. Consequently, the optimizer is forced to allocate the 0◦ GFRP UD candidate on the webs of the structure in order to also place them on the desirable top and bottom faces. The consequence of this is particularly pronounced for the parameterization with foam as a candidate material. In this case, the optimizer cannot allocate the same amount of foam on the webs as in the case of the Long-Long parameterization; ultimately resulting in a substantial increase of the final mass. Naturally surpassed by the 0◦ GFRP UD candidate, the −45◦ GFRP UD candidate is the second most present candidate. This candidate may very well represent beneficial properties to constrain the risk of buckling. The −45◦ GFRP UD candidate occurs in particular at the tip section where the pressure load is introduced, hence making this area prone to local buckling. The thickness is smallest at the tip section and largest between the tip and the mid-section as this region is vulnerable to buckling along the pressure side as well. Notice that the thickness is changed with at most two ply thicknesses between neighboring geometry domains, satisfying the constraints on thickness variation rate (MC2), see (7). 5.3 General performance of the DMTO approach The capabilities of the suggested DMTO approach have been demonstrated on differently parameterized numerical examples of a main spar. The suggested SLP approach is found robust, providing near-discrete designs in an acceptable number of iterations. Simple rounding finalizes the designs, causing average structural criteria constraint perturbations < 3%, which is deemed acceptable. However, for the Grid-Long and Grid-Circ parameterizations with foam, rounding causes infeasible manufacturing constraints on contiguity. The considered parameterizations with and without foam as a candidate do indeed give an insight into the relation between weight saving and design complexity. In the considered load case, foam is consistently an advantageous candidate. The lightest design, weighing 1163kg prior to rounding, occurred on basis of the quite complex Grid-Grid parameterization with foam, difficult if not impossible to realize with today’s manufacturing techniques. In contrast, the simple Circ-Circ parameterization with foam proved inadequate for the considered load case, weighing 30.6% more than the Grid-Grid parameterization. Nevertheless, the least complex result with foam of all, being the Long-Long parameterization, ended up weighing 1250kg prior to rounding, i.e., merely 7.5% more than the complex Grid-Grid parameterization. The relation between weight saving and complexity is hence not straightforward. Complex parameterizations with great design freedom result in the largest weight savings, but are hardly manufacturable. However, fairly simple, but well-parameterized, designs may likewise per- 20 form well. The results in general appear to provide great found as a great source of inspiration for manufacturable inspiration for detailed post-processing. This is the exact thickness variation and stacking sequences throughout the structure; inspiration for detailed post-processing that intention of the suggested DMTO method. may very well outperform intuition, exploiting elastic couplings that may appear obscure at first glance. 6 Conclusion In this work, we have presented a gradient based topology optimization method for minimizing the mass of largescale laminated composite structures. The method is labelled DMTO for Discrete Material and Thickness Optimization. The DMTO method enables minimum mass designs by simultaneously determining an optimum material distribution and thickness variation. This is done while also considering industrially relevant constraints on structural performance i.e., buckling load factors, eigenfrequencies, and limited displacements. Furthermore, common design guidelines or rules, referred to as manufacturing constraints, are included explicitly as series of linear inequalities. The capabilities of the method have been demonstrated on a generic main spar used in many designs of wind turbine blades. In order to give insight into the relation between potential weight saving and design complexity, the main spar was parameterized in different ways ranging from simple to complex to manufacture with today’s production techniques in mind. The results show that some parameterizations can indeed obtain significant weight savings while also being simple to manufacture. It is thus stressed that the initial parameterization is of great importance as both the performance and the manufacturability depend hereupon. The design of the main spar together with the applied flap-wise bending load case makes foam material an attractive candidate. The results showed that, on average, examples with foam as a candidate obtained a final mass, nearly 30% lower than those without foam as a candidate. The preceding work by Sørensen and Lund (2013) suggests that SLP methods are favorable compared to e.g., SQP formulations. This is mainly due to the nature of the manufacturing constraint for preventing intermediate void through the thickness of the laminate. Compared to the preceding work, we are now dealing with a far more difficult problem given structural performance constraints with sensitivities of both operational signs. An SLP merit function approach, based on Svanberg (2004), was applied to pose unconditionally feasible LP problems. The SLP approach was found robust and effective, emphasized by the fact that all of the numerical examples converged to feasible designs within 28-142 iterations. A three-step continuation approach with increasing penalization in a product of RAMP interpolation schemes was found efficient for obtaining near-discrete designs. Strictly binary designs were obtained through finalization by simple rounding, resulting in constraint perturbations < 3% in most cases. In general, the DMTO method is Acknowledgements This work was supported by the Danish Centre for Composite Structures and Materials for Wind Turbines (DCCSM), grant no. 09-067212 from the Danish Strategic Research Council (DSF), and by the Danish Research Council for Technology and Production Sciences (FTP), grant no. 10-082695. This support is gratefully acknowledged. The authors thank Mathias Stolpe, Technical University of Denmark, Department of Wind Energy, for fruitful discussions and inputs for this research. The final publication is available at Springer via http://dx.doi.org/10.1007/s00158-014-1047-5 References Ahmad, S., Irons, B. M., and Zienkiewicz, O. C. Analysis of thick and thin shell structures by curved elements. International Journal for Numerical Methods in Engineering, 2:419–451, 1970. Arora, J. S. Introduction to Optimum Design. Elsevier Academic Press, 2 edition, 2004. ISBN 0120641550. Arora, J. and Wang, Q. Review of formulations for structural and mechanical system optimization. Structural and Multidisciplinary Optimization, 30(4):251– 272, 2005. ISSN 1615-147X. Bendsøe, M. P. Optimal shape design as a material distribution problem. Structural and Multidisciplinary Optimization, 1(4):193–202, 1989. Bendsøe, M. P. and Sigmund, O. Topology Optimization. Springer Verlag, second edition, 2003. ISBN 3-54042992-1. Bruggi, M. and Duysinx, P. Topology optimization for minimum weight with compliance and stress constraints. Structural and Multidisciplinary Optimization, 46(3):369–384, 2012. ISSN 1615-147X. Bruyneel, M. SFP-a new parameterization based on shape functions for optimal material selection: application to conventional composite plies. Structural and Multidisciplinary Optimization, 43(1):17–27, JAN 2011. ISSN 1615-147X. Bruyneel, M., Beghin, C., Craveur, G., Grihon, S., and Sosonkina, M. Stacking sequence optimization for constant stiffness laminates based on a continuous opti- 21 mization approach. Structural and Multidisciplinary Optimization, 46(6):783–794, 2012. ISSN 1615-147X. volume 1. John Wiley & Sons, New York, 2010. ISBN 978-0-470-97271-7. Bruyneel, M., Duysinx, P., Fleury, C., and Gao, T. Ex- Kennedy, G. J. and Martins, J. R. R. A. A laminate tensions of the Shape Functions with Penalization Paparametrization technique for discrete ply-angle probrameterization for Composite-Ply Optimization. AIAA lems with manufacturing constraints. Structural and Journal, 49(10):2325–2329, OCT 2011. ISSN 0001Multidisciplinary Optimization, 2013. 1452. Kim, C., Song, S., Hwang, W., Park, H., and Han, K. Costin, D. P. and Wang, B. P. Optimum design of a comOn the failure indices of quadratic failure criteria for posite structure with manufacturing constraints. Thinoptimal stacking sequence design of laminated plate. Walled Structures, 17(3):185–202, 1993. Applied Composite Materials, 1(1):81–85, 1994. ISSN 0929-189X. Courant, R. and Hilbert, D. Methods of mathematical physics, volume 1. Interscience Publishers, New York, Le, C., Norato, J., Bruns, T., Ha, C., and Tortorelli, D. 1953. Stress-based topology optimization for continua. StrucDuysinx, P. and Sigmund, O. New development in hantural and Multidisciplinary Optimization, 41(4):605– dling stress constraints in optimal material distribu620, 2010. ISSN 1615-147X. tion. In 7th Symposium on Multidisciplinary Analysis and Optimization., pages 1501–1509, 1998. AIAA-98- Le Riche, R. and Haftka, R. T. Optimization of laminate stacking sequence for buckling load maximization by 4906. genetic algorithm. AIAA, 31(5):951–956, May, 1993. Gao, T., Zhang, W., and Duysinx, P. A bi-value coding parameterization scheme for the discrete optimal orien- Lindgaard, E. and Dahl, J. On compliance and buckling tation design of the composite laminate. International objective functions in topology optimization of snapJournal for Numerical Methods in Engineering, 91(1): through problems. Structural and Multidisciplinary 98–114, 2012. ISSN 1097-0207. Optimization, 47(3):409–421, 2012. Ghiasi, H., Pasini, D., and Lessard, L. Optimum stackLindgaard, E. and Lund, E. Nonlinear buckling optimizaing sequence design of composite materials Part I: Contion of composite structures. Computer Methods in Apstant stiffness design. Composite Structures, 90(1):1– plied Mechanics and Engineering, 199(37-40):2319– 11, 9 2009. 2330, 2010. ISSN 0045-7825. Ghiasi, H., Fayazbakhsh, K., Pasini, D., and Lessard, L. Optimum stacking sequence design of composite mate- Liu, B., Haftka, R. T., Akgün, M. A., and Todoroki, A. Permutation genetic algorithm for stacking sequence rials Part II: Variable stiffness design. Composite Strucdesign of composite laminates. Computer Methods tures, 93(1):1–13, 12 2010. in Applied Mechanics and Engineering, 186:357–372, Gill, P., Murray, W., and Saunders, M. SNOPT: An March 1999. SQP algorithm for large-scale constrained optimizaLiu, D., Toropov, V. V., Querin, O. M., and Barton, D. C. tion. SIAM Review, 47(1):99–131, 2005. Bilevel Optimization of Blended Composite Wing PanGroenwold, A. and Haftka, R. Optimization with nonels. Journal Of Aircraft, 48(1):107–118, JAN-FEB homogeneous failure criteria like tsai-wu for composite 2011. ISSN 0021-8669. laminates. Structural and Multidisciplinary Optimization, 32(3):183–190, 2006. ISSN 1615-147X. Lund, E. Finite element based design sensitivity analysis and optimization. Ph.D. Thesis, Institute of MechanHvejsel, C. and Lund, E. Material interpolation schemes ical Engineering, Aalborg University, Denmark, 1994. for unified topology and multi-material optimization. Special report no. 23. Structural and Multidisciplinary Optimization, 43(6): 811–825, 2011. Lund, E. Buckling topology optimization of laminated multi-material composite shell structures. Composite Hvejsel, C., Lund, E., and Stolpe, M. Optimization strateStructures, 91(2):158–167, NOV 2009. ISSN 0263gies for discrete multi-material stiffness optimization. 8223. Structural and Multidisciplinary Optimization, 44(2): 149–163, 2011. Kassapoglou, C. Design and Analysis of Composite Structures: With Applications to Aerospace Structures, Lund, E. and Stegmann, J. On structural optimization of composite shell structures using a discrete constitutive parametrization. Wind Energy, 8(1):109–124, 2005. 22 Lund, E., Sørensen, R., and Sørensen, S. N. Multiblended laminates. Composites Part B: Engineering, criteria multi-material topology optimization of lami38(4):469–480, 6 2007. nated composite structures including local constraints. In Book of Abstracts, Orlando, Florida, 2013. 10th Seyranian, A., Lund, E., and Olhoff, N. Multiple eigenvalues in structural optimization problems. Structural World Congress on Structural and Multidisciplinary Optimization, 8:207–227, 1994. Optimization. Manne, P. M. and Tsai, S. W. Design Optimization of Sørensen, S. N. and Lund, E. Topology and thickness optimization of laminated composites including manuComposite Plates: Part II–Structural Optimization by facturing constraints. Structural and Multidiciplinary Plydrop Tapering. Journal of Composite Materials, 32 Optimization, 48:249–265, 2013. (6):572–598, March 01 1998. MUST. The MUltidisciplinary Synthesis Tool, 2013. Stegmann, J. and Lund, E. Discrete material optimization of general composite shell structures. Internahttp://www.must.m-tech.aau.dk. tional Journal for Numerical Methods in Engineering, 62(14):2009–2027, 2005. Nemhauser, G. L. and Wolsey, L. A. Integer and Combinatorial Optimization. John Wiley & Sons, Inc, 1988. Stolpe, M. and Svanberg, K. An alternative interpolation ISBN 0-471-82819-X. scheme for minimum compliance topology optimization. Structural and Multidisciplinary Optimization, 22 Neves, M., Rodrigues, H., and Guedes, J. Generalized (2):116–124, 2001. topology design of structures with a buckling load criterion. Structural Optimization, 10:71–78, 1995. Svanberg, K. The method of moving asymptotes - a new method for structural optimization. International JourNiu, B., Olhoff, N., Lund, E., and Cheng, G. Discrete nal for Numerical Methods in Engineering, 24(2):359– material optimization of vibrating laminated compos373, February 1987. ite plates for minimum sound radiation. International Journal of Solids and Structures, 47(16):2097–2114, Svanberg, K. Some modelling aspects for the fortran imAUG 1 2010. ISSN 0020-7683. plementation of MMA. Technical report, 2004. Olhoff, N., Bendsøe, M. P., and Rasmussen, J. On cadintegrated structural topology and design optimization. Toropov, V. V., Jones, R., Willment, T., and Funnell, M. Weight and Manufacturability Optimization of ComComputer Methods in Applied Mechanics and Engiposite Aircraft Components Based on a Genetic Algoneering, 89(1):259–279, 1991. rithm. In Proceedings of 6th World Congress of Structural and Multidisciplinary Optimization (WCSMO). Overgaard, L., Lund, E., and Thomsen, O. Structural colRio de Janeiro, Brazil, May–June 2005. lapse of a wind turbine blade. Part A: Static test and equivalent single layered models. Composites Part A: Applied Science and Manufacturing, 41(2):257 – 270, Tsai, S. W. and Wu, E. M. A general theory of strength for anisotropic materials. Journal of Composite Materials, 2010. ISSN 1359-835X. 5(1):58–80, 1971. Panda, S. and Natarajan, R. Analysis of laminated comWittrick, W. Rates of change of eigenvalues, with referposite shell structures by finite element method. Comence to buckling and vibration problems. Journal of the puters & Structures, 14(3-4):225–230, 1981. Royal Aeronautical Society, 66:590–591, 1962. Parı́s, J., Navarrina, F., Colominas, I., and Casteleiro, M. Zein, S., Colson, B., and Grihon, S. A primal-dual backBlock aggregation of stress constraints in topology optracking optimization method for blended composite timization of structures. Advances in Engineering Softstructures. Structural and Multidisciplinary Optimizaware, 41:433–441, 2010. tion, 45(5):669–680, MAY 2012. ISSN 1615-147X. Rietz, A. Sufficiency of a finite exponent in simp (power Zhou, M. and Fleury, R. Composite Optimization law) methods. Structural and Multidisciplinary OptiPly Drop-Rate Constraints for Concepts and Detailed mization, 21(2):159–163, 2001. Design. In Proceedings of the 23rd International Congress of Theoretical and Applied Mechanics (ICRodrigues, H., Guedes, J., and Bendsøe, M. Necessary TAM). Beijing, China, August 2012. conditions for optimal design of structures with a nonsmooth eigenvalue based criterion. Structural OptimizaZhou, M., Fleury, R., and Kemp, M. Optimization of tion, 9:52–56, 1995. Composits - Recent Advances and Application. The 7th Altair CAE Technology Conference, Altair, 2011. Seresta, O., Gürdal, Z., Adams, D. B., and Watson, L. T. Optimal design of composite wing structures with 23